#------------------------------------------------------------------------------
#$Date: 2016-03-26 14:08:46 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180249 $
#$URL: svn://www.crystallography.net/cod/cif/7/11/35/7113567.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7113567
loop_
_publ_author_name
'Rather, Beth'
'Zaworotko, Michael J.'
_publ_section_title
;
 A 3D metal-organic network, [Cu2(glutarate)2(4,4′-bipyridine)],
 that exhibits single-crystal to single-crystal dehydration and
 rehydrationElectronic supplementary information (ESI) available:
 experimental details, IR, TGA and XRPD of all compounds. See
 http://www.rsc.org/suppdata/cc/b3/b301219k/.
;
_journal_issue                   7
_journal_name_full               'Chemical Communications'
_journal_page_first              830
_journal_paper_doi               10.1039/b301219k
_journal_year                    2003
_chemical_formula_moiety         '(C22 H24 Cu2 N2 O8)n,5n(H2 O1)'
_chemical_formula_sum            'C22 H24 Cu2 N2 O13'
_chemical_formula_weight         651.51
_chemical_name_systematic
; 
? 
;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 91.473(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   24.238(2)
_cell_length_b                   13.0527(13)
_cell_length_c                   8.6313(8)
_cell_measurement_reflns_used    4845
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      27.44
_cell_measurement_theta_min      2.86
_cell_volume                     2729.8(4)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.984
_diffrn_measured_fraction_theta_max 0.984
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0286
_diffrn_reflns_av_sigmaI/netI    0.0370
_diffrn_reflns_limit_h_max       30
_diffrn_reflns_limit_h_min       -30
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            8295
_diffrn_reflns_theta_full        27.48
_diffrn_reflns_theta_max         27.48
_diffrn_reflns_theta_min         1.68
_exptl_absorpt_coefficient_mu    1.625
_exptl_absorpt_correction_T_max  1.000
_exptl_absorpt_correction_T_min  0.858
_exptl_absorpt_correction_type   SADABS
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    1.585
_exptl_crystal_density_meas      0
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       diamondoid
_exptl_crystal_F_000             1328
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.07
_exptl_crystal_size_min          0.05
_refine_diff_density_max         0.594
_refine_diff_density_min         -0.417
_refine_diff_density_rms         0.086
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.049
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     222
_refine_ls_number_reflns         3082
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.049
_refine_ls_R_factor_all          0.0484
_refine_ls_R_factor_gt           0.0410
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0358P)²+11.6842P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0941
_refine_ls_wR_factor_ref         0.0972
_reflns_number_gt                2722
_reflns_number_total             3082
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            b301219k.txt
_cod_data_source_block           compound2a
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to
/usr/data/users/saulius/automatic-downloads/retrospective/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 
;
_cod_original_cell_volume        2729.8(5)
_cod_original_sg_symbol_H-M      C2/c
_cod_database_code               7113567
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Cu1 Cu 0.205251(14) 0.20430(3) 0.44606(4) 0.01417(11) Uani 1 1 d .
N1 N 0.13951(9) 0.13937(18) 0.3045(3) 0.0161(5) Uani 1 1 d .
O1 O 0.25668(9) 0.57640(15) 0.9927(2) 0.0215(4) Uani 1 1 d .
O2 O 0.18014(9) 0.65457(16) 0.9084(3) 0.0231(5) Uani 1 1 d .
O3 O 0.17339(9) 0.21662(17) 0.6536(2) 0.0259(5) Uani 1 1 d .
O4 O 0.25045(9) 0.29039(16) 0.7429(2) 0.0222(4) Uani 1 1 d .
C1 C 0.20882(12) 0.5758(2) 0.9326(3) 0.0171(6) Uani 1 1 d .
C2 C 0.18388(13) 0.4753(2) 0.8800(3) 0.0222(6) Uani 1 1 d .
H2A H 0.1973 0.4597 0.7753 0.027 Uiso 1 1 calc R
H2B H 0.1433 0.4838 0.8710 0.027 Uiso 1 1 calc R
C3 C 0.19634(13) 0.3840(2) 0.9847(3) 0.0201(6) Uani 1 1 d .
H3A H 0.1784 0.3942 1.0854 0.024 Uiso 1 1 calc R
H3B H 0.2367 0.3794 1.0047 0.024 Uiso 1 1 calc R
C4 C 0.17566(13) 0.2840(2) 0.9113(3) 0.0200(6) Uani 1 1 d .
H4A H 0.1837 0.2267 0.9835 0.024 Uiso 1 1 calc R
H4B H 0.1351 0.2880 0.8952 0.024 Uiso 1 1 calc R
C5 C 0.20203(12) 0.2618(2) 0.7574(3) 0.0175(6) Uani 1 1 d .
C6 C 0.14480(12) 0.0455(2) 0.2452(3) 0.0192(6) Uani 1 1 d .
H6 H 0.1743 0.0035 0.2821 0.023 Uiso 1 1 calc R
C7 C 0.10891(12) 0.0069(2) 0.1318(3) 0.0221(6) Uani 1 1 d .
H7 H 0.1140 -0.0603 0.0926 0.027 Uiso 1 1 calc R
C8 C 0.06572(12) 0.0669(2) 0.0762(3) 0.0201(6) Uani 1 1 d .
C9 C 0.06086(12) 0.1641(2) 0.1360(3) 0.0206(6) Uani 1 1 d .
H9 H 0.0320 0.2080 0.1000 0.025 Uiso 1 1 calc R
C10 C 0.09809(12) 0.1974(2) 0.2484(3) 0.0199(6) Uani 1 1 d .
H10 H 0.0942 0.2649 0.2879 0.024 Uiso 1 1 calc R
C11 C 0.02388(13) 0.0254(3) -0.0404(3) 0.0248(7) Uani 1 1 d .
H11A H 0.0419 -0.0251 -0.1081 0.030 Uiso 1 1 calc R
H11B H 0.0097 0.0821 -0.1064 0.030 Uiso 1 1 calc R
O1W O 0.4936(4) 0.8438(14) 0.6260(14) 0.125(6) Uani 0.40 1 d P
O2W O 0.568(2) 0.833(6) 0.591(6) 0.14(2) Uani 0.20 1 d P
O3W O 0.5147(8) 0.9178(12) 0.395(2) 0.138(6) Uani 0.40 1 d P
O4W O 0.4521(7) 0.9358(16) 0.391(3) 0.147(10) Uani 0.30 1 d P
O5W O 0.548(2) 0.768(4) 0.675(6) 0.18(2) Uani 0.30 1 d P
O6W O 0.5000 0.9251(17) 0.2500 0.22(2) Uani 0.40 2 d SP
O7W O 0.5626(12) 0.907(2) 0.493(5) 0.123(11) Uani 0.20 1 d P
O8W O 0.5519(6) 0.794(3) 0.632(2) 0.126(12) Uani 0.50 1 d P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O2 Cu1 O1 168.11(9) 6_565 4_546
O2 Cu1 O3 86.97(9) 6_565 .
O1 Cu1 O3 90.98(10) 4_546 .
O2 Cu1 O4 90.18(9) 6_565 7_556
O1 Cu1 O4 89.45(9) 4_546 7_556
O3 Cu1 O4 168.13(9) . 7_556
O2 Cu1 N1 93.06(9) 6_565 .
O1 Cu1 N1 98.79(9) 4_546 .
O3 Cu1 N1 104.21(9) . .
O4 Cu1 N1 87.43(9) 7_556 .
O2 Cu1 Cu1 83.24(6) 6_565 7_556
O1 Cu1 Cu1 85.01(6) 4_546 7_556
O3 Cu1 Cu1 88.86(6) . 7_556
O4 Cu1 Cu1 79.36(6) 7_556 7_556
N1 Cu1 Cu1 166.25(6) . 7_556
C6 N1 C10 117.4(2) . .
C6 N1 Cu1 120.07(19) . .
C10 N1 Cu1 121.25(19) . .
C1 O1 Cu1 122.38(18) . 4_556
C1 O2 Cu1 124.92(19) . 6_566
C5 O3 Cu1 117.40(19) . .
C5 O4 Cu1 128.98(19) . 7_556
O2 C1 O1 124.3(3) . .
O2 C1 C2 116.5(3) . .
O1 C1 C2 119.2(3) . .
C1 C2 C3 115.5(2) . .
C2 C3 C4 111.4(2) . .
C5 C4 C3 112.7(2) . .
O4 C5 O3 124.9(3) . .
O4 C5 C4 116.9(2) . .
O3 C5 C4 118.3(3) . .
N1 C6 C7 122.6(3) . .
C8 C7 C6 119.7(3) . .
C9 C8 C7 117.6(3) . .
C9 C8 C11 121.2(3) . .
C7 C8 C11 121.2(3) . .
C8 C9 C10 119.6(3) . .
N1 C10 C9 123.2(3) . .
C8 C11 C11 110.9(3) . 5
O8W O1W O5W 18(3) . .
O8W O2W O5W 10(3) . .
O8W O2W O7W 140(7) . .
O5W O2W O7W 149(5) . .
O6W O3W O7W 142(2) . .
O6W O3W O4W 73.9(16) . .
O7W O3W O4W 144(2) . .
O3W O4W O6W 46.5(10) . .
O8W O5W O2W 14(5) . .
O8W O5W O1W 67(5) . .
O2W O5W O1W 77(3) . .
O3W O6W O3W 172(3) 2_655 .
O3W O6W O4W 59.6(12) 2_655 2_655
O3W O6W O4W 121.2(12) . 2_655
O3W O6W O4W 121.2(12) 2_655 .
O3W O6W O4W 59.6(12) . .
O4W O6W O4W 171(2) 2_655 .
O2W O7W O3W 123(3) . .
O5W O8W O2W 156(7) . .
O5W O8W O1W 96(6) . .
O2W O8W O1W 102(7) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Cu1 O2 1.965(2) 6_565
Cu1 O1 1.973(2) 4_546
Cu1 O3 1.975(2) .
Cu1 O4 1.977(2) 7_556
Cu1 N1 2.157(2) .
Cu1 Cu1 2.6253(7) 7_556
N1 C6 1.335(4) .
N1 C10 1.339(4) .
O1 C1 1.259(4) .
O1 Cu1 1.973(2) 4_556
O2 C1 1.256(3) .
O2 Cu1 1.965(2) 6_566
O3 C5 1.265(3) .
O4 C5 1.241(4) .
O4 Cu1 1.977(2) 7_556
C1 C2 1.509(4) .
C2 C3 1.522(4) .
C3 C4 1.530(4) .
C4 C5 1.516(4) .
C6 C7 1.387(4) .
C7 C8 1.383(4) .
C8 C9 1.376(4) .
C8 C11 1.510(4) .
C9 C10 1.378(4) .
C11 C11 1.519(6) 5
O1W O8W 1.55(3) .
O1W O5W 1.68(4) .
O2W O8W 0.74(7) .
O2W O5W 1.23(9) .
O2W O7W 1.29(6) .
O3W O6W 1.292(19) .
O3W O7W 1.43(4) .
O3W O4W 1.53(3) .
O4W O6W 1.71(2) .
O5W O8W 0.52(8) .
O6W O3W 1.292(19) 2_655
O6W O4W 1.71(2) 2_655
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
C1 C2 C3 C4 -172.7(3)
C2 C3 C4 C5 60.1(3)
